# Question 8.3: Design of a Fatigue-Resistant Shaft Your company has produce......

Design of a Fatigue-Resistant Shaft
Your company has produced several thousand shafts that have a fatigue strength of 20,000 psi. The shafts are subjected to high bending loads during rotation. Your sales engineers report that the first few shafts placed into service failed in a short period of time by fatigue. Design a process by which the remaining shafts can be salvaged by improving their fatigue properties.

Step-by-Step
The 'Blue Check Mark' means that this solution was answered by an expert.

Fatigue failures typically begin at the surface of a rotating part; thus, increasing the
strength at the surface improves the fatigue life of the shaft. A variety of methods might be used to accomplish this.
If the shaft is made from steel, we could carburize the surface of the part (Chapter 5). In carburizing, carbon is diffused into the surface of the shaft. After an appropriate heat treatment, the higher carbon content at the surface increases the strength of the surface and, perhaps more importantly, introduces compressive residual stresses at the surface.
We might consider cold working the shaft; cold working increases the yield strength of the metal and, if done properly, introduces compressive residual stresses. The cold work also reduces the diameter of the shaft and, because of the dimensional change, the shaft may not be able to perform its function.
Another alternative is to shot peen the shaft. Shot peening introduces local compressive residual stresses at the surface without changing the dimensions of the part. This process, which is also inexpensive, might be sufficient to salvage the remaining shafts.

Question: 8.6

## Design of a Process to Produce a Copper Strip We want to produce a 0.1-cm-thick, 6-cm-wide copper strip having at least 60,000 psi yield strength and at least 5% elongation. We are able to purchase 6-cm-wide strip only in thicknesses of 5 cm. Design a process to produce the product we need, but in ...

In Example 8-5, we relied on a series of cold work...
Question: 8.5

## Design of a Process to Produce Copper Strip We wish to produce a 0.1-cm-thick, 6-cm-wide copper strip having at least 60,000 psi yield strength and at least 5% elongation. We are able to purchase 6-cm-wide strip only in a thickness of 5 cm. Design a process to produce the product we need. Refer to ...

In Example 8-2, we found that the required propert...
Question: 8.4

## Design of a Wire-Drawing Process Design a process to produce 0.20-in.-diameter copper wire. The mechanical properties of the copper to be considered are shown in Figure 8-6. ...

Wire drawing is the obvious manufacturing techniqu...
Question: 8.2